Macromolecules 2003, 36, 685-691
Crystal Structure of the Clathrate Form of Syndiotactic Poly(m-methylstyrene) Containing Carbon Disulfide Vittorio Petraccone,* Oreste Tarallo, and Valeria Califano Dipartimento di Chimica, Universita` degli Studi di Napoli “Federico II”, Complesso di Monte Sant’Angelo, Via Cintia, 80126 Napoli, Italy Received August 12, 2002; Revised Manuscript Received October 17, 2002
ABSTRACT: The crystal structure of the clathrate form of syndiotactic poly(m-methylstyrene) containing carbon disulfide is presented. The structure is characterized by polymer chains in s(2/1)2 helical conformation and CS2 molecules packed in an orthorhombic unit cell with axes a ) 17.8 Å, b ) 13.1 Å, and c ) 7.8 Å, according to the space group Pcaa. The calculated crystalline density is 1.14 g/cm3 for two polymer chains (eight monomer units) and four carbon disulfide molecules included in the unit cell. As in the packing model proposed for the crystal structures of the β class of the syndiotactic poly(pmethylstyrene) clathrates, the guest molecules occupy cavities delimited by isomorphous helices along the b axis and are related by the crystallographic 2-fold screw axis of the unit cell. The packing of the helices along the a axis, instead, is similar to the close packing realized by the chains only in the clathrates and in the δ form of syndiotactic polystyrene.
Introduction Recently, homogeneous catalytic systems, based on titanium or zirconium compounds and methylalumoxane, have allowed producing highly syndiotactic polystyrene (s-PS)1 and substituted polystyrenes.2 Some of these polymers have shown the interesting property of cocrystallizing with low molecular weight substances to form polymeric clathrates. Clathrate structures have been first described for s-PS,3 and the crystal structure of the clathrate forms containing toluene,4 iodine,5 and 1,2-dichloroethane6 have been completely characterized. Moreover, for this polymer some promising applications have been suggested in the field of chemical separations, in particular for water or air purification from volatile organic compounds.7 This possibility is mainly due to the existence of the δ crystalline form,8 which is nanoporous and can be obtained by removal of guest molecules from clathrate samples by suitable solvent treatments.9 Subsequently, other syndiotactic styrenic polymers, such as p-methylstyrene (s-PPMS)10-12 and m-methylstyrene (s-PMMS),13 have been studied, and their property of cocrystallizing with low molecular weight compounds to give clathrate structures has been also pointed out. Up to now, detailed crystalline structures of clathrate forms of s-PPMS including tetrahydrofuran (THF),14 o-dichlorobenzene (o-DCB),15 and benzene16 have been described, while no crystalline structure of s-PMMS clathrate forms has been proposed yet. Obtaining clathrate forms has been also considered for co-syndiotactic copolymers of styrene and other substituted styrenic monomers, such as p-methylstyrene,17 in order to modulate the dimension of the cavity in which guest molecules are hosted as a function of the copolymer composition. A common feature of all the clathrate forms that have been studied is that the polymer chains assume the same s(2/1)2 helical conformation, with a repetition period of 7.7-7.8 Å. As far as the shape of the cavity is concerned, structural studies on the clathrate forms of s-PS and s-PPMS indicate that two different types of cavity containing guest molecules are possible.18 In the
Figure 1. X-ray fiber diffraction pattern of the clathrate form of s-PMMS containing carbon disulfide. Small amounts of form I are revealed by the reflections at 2θ ) 15.1° (indicated by an arrow) on the first layer line corresponding to the strongest reflections of that form, whose spectrum is reported in ref 13.
case of s-PS,4-6 only one kind of centrosymmetric cavity delimited by eight benzene rings of two enantiomorphous adjacent polymer chains has been found. In the case of s-PPMS, instead, in addition to the formerly described cavity (proposed for the clathrate form of s-PPMS with o-DCB15), a different type of cavity has been found for THF14 and benzene16 clathrates, in which cavities are arranged around 2-fold screw axes of the lattice and delimited by four benzene rings of one polymer chain and two benzene rings of the adjacent isomorphous one. Consequently, the terms R class and β class have been introduced in order to differentiate clathrate forms containing the first type of cavity from those containing the second type.12 In this paper, for the first time, the crystal structure of a clathrate form of s-PMMS is presented. Our aim is to make a comparison between the clathrate structure of this homopolymer with those of s-PS and s-PPMS, also in order to allow the analysis of the influence of m-methylstyrene comonomeric units in co-syndiotactic copolymers with styrene.
10.1021/ma021313c CCC: $25.00 © 2003 American Chemical Society Published on Web 01/08/2003
Petraccone et al.
Macromolecules, Vol. 36, No. 3, 2003 Table 1. Diffraction Angles (2θ), Bragg Distances (dobs), and Intensities (Iobs) in Arbitrary Units (AU) of the Reflections Observed on the Layer Lines (l) of the X-ray Fiber Diffraction Pattern of the Clathrate Form of s-PMMS Containing Carbon Disulfide of Figure 1 l 0 0 0 0 0 0 0 0 0 0 0 0 1
Figure 2. Two possible conformers of the s-PMMS helical chains with symmetry s(2/1)2.
Experimental Part and Calculation Methods s-PMMS was prepared using an homogeneous catalytic system based on pentamethylcyclopentadienyltitanium trichloride (Cp*TiCl3) and methylalumoxane (MAO) in toluene according to the procedure described in ref 13. The syndiotacticity of the insoluble fraction in 2-butanone determined by 13 C NMR was very high ([rrrr] > 95%).
2θ (deg) dobs (Å) Iobs (AU) 6.82 10.0 12.4 13.4 16.8 20.2 22.7 27.0 28.8 30.7 33.8 40.6 14.2
13.0 8.85 7.14 6.61 5.28 4.40 3.92 3.30 3.10 2.91 2.65 2.22 6.24
4394 1107 3856 564 2693 1215 266 266 87 652 187 1077
l 1 1 1 1 1 2 2 2 2 2 2 2 2
2θ (deg) dobs (Å) Iobs (AU) 18.2 20.2 23.6 28.8 39.5 24.7 26.4 28.3 30.7 33.1 37.1 41.4 43.7
4.87 4.40 3.77 3.10 2.28 3.60 3.38 3.15 2.91 2.71 2.42 2.18 2.07
1598 4602 1823 269 335 631 249 1892 306 203 102 462 236
Unoriented samples of s-PMMS clathrate containing carbon disulfide were obtained by swelling at room temperature amorphous specimens prepared in a hot press by melting asprepared samples at 225 °C and successive quenching in icewater. Oriented clathrate specimens were obtained by swelling fibers, in the mesomorphic form III, into CS2 for 48 h, keeping fixed the ends of the specimen. Fibers of the mesomorphic form III were obtained by drawing amorphous samples with a miniature mechanical tester apparatus (Reometric Scientific Minimat) at a drawing rate of 10 mm/min at a temperature in the range 85-90 °C.
Figure 3. ab projection of the packing model of the s-PMMS chains according to space group Pcaa. The crystallographic symmetry elements of the space group are shown. The approximate z/c fractional coordinates of the barycenters of the phenyl rings are also shown.
Macromolecules, Vol. 36, No. 3, 2003
Figure 4. Packing model proposed for the crystal structure of the s-PMMS clathrate containing carbon disulfide, in the space group Pcaa: ab projection (a) and bc projection (b). The approximated z/c fractional coordinates of the barycenters of the phenyl rings are shown. R ) right-handed, L ) left-handed helices. The shortest nonbonded distances (less than 4.0 Å) are indicated. In (b) only a couple of polymer chains, along the b axis, are reported. The oriented clathrate samples were sealed in a Lyndemann glass capillary soon after swelling in order to avoid the removal of the solvent that would cause them to transform rapidly into form I. Wide-angle X-ray diffraction patterns of unoriented samples were obtained with nickel-filtered Cu KR radiation with an automatic Philips powder diffractometer. The X-ray fiber diffraction patterns of oriented samples were obtained on a BAS-MS imaging plate (FUJIFILM) with a cylindrical camera (radius 57.3 mm, Ni-filtered Cu KR radiation monochromatized with a graphite crystal) and processed with a digital scanner (FUJI-BAS 1800). Calculated structure factors were obtained as Fcalc ) (∑|Fi|2Mi)1/2, where Mi is the multiplicity factor and the summation is taken over all reflections included in the 2θ range of the corresponding spot observed in the X-ray fiber diffraction pattern. A thermal factor (B ) 8 Å2) and atomic scattering factors from ref 19 were used. The observed structure factors Fobs were evaluated from the intensities of the reflections observed in the X-ray fiber diffraction pattern
(Iobs) as Fobs ) (Iobs/Lp)1/2, where Lp is the Lorentz polarization factor for X-ray fiber diffraction:
0.5(cos2 2θ + cos2 2θM) 1 + cos2 2θM
0.5(1 + cos 2θM + cos2 2θ) 1 + cos 2θM
(sen2 2θ - ζ2)1/2
with 2θM ) 26.6° the inclination angle of the monochromator and ζ ) λ(l/c), l and c being the order of the layer line and the chain axis periodicity, respectively, and λ the wavelength of the used radiation (1.5418 Å). The observed intensities Iobs were evaluated integrating the crystalline peaks observed in the X-ray diffraction profiles, read along different layer lines, after the subtraction of the amorphous contribution due to sample and glass capillary. Owing to the different shapes of the reflection on the equator and on the first and second layer lines, due to the different dimensions of the lamellar crystals in the direction perpendicular and parallel to the chain axis,
Petraccone et al.
Macromolecules, Vol. 36, No. 3, 2003
Table 2. Fractional Coordinates of the Atoms of an Asymmetric Unit of the Model Proposed (Figure 4) for the Clathrate Form of s-PMMS with Carbon Disulfidea C1 C2 C3 C4 C5 C6 C7 C8 C9 C10 C11 S
0.343 0.297 0.250 0.352 0.409 0.459 0.454 0.398 0.348 0.392 0.250 0.337
0.000 0.068 0.004 0.137 0.099 0.165 0.271 0.311 0.243 0.426 0.285 0.285
0.250 0.373 0.500 0.465 0.571 0.650 0.624 0.520 0.443 0.490 0.000 -0.019
aHydrogen atoms were included in the structure factors calculation, but they are omitted in this table for simplicity.
different factors have been used to scale the observed and calculated structure factors on the diverse layer lines. The discrepancy factor R has been evaluated as
taking into account only the observed reflections. Energy calculations were carried out by using commercially available software (Cerius2 version 4.2 by Accelrys Inc.). The force field used was the Compass Force Field.20 The starting conformations of the s-PMMS polymer chains correspond to the conformations found by molecular mechanics calculations
Figure 5. Trend of the discrepancy factor (R) vs the occupancy factor. by De Rosa et al.21 These conformations do not present relevant differences in the internal parameters with respect to those proposed for s-PS and s-PPMS chains in the clathrate structures reported in the literature. The C-S bond length and the S-C-S angle of the carbon disulfide molecules were assumed to be respectively 1.55 Å and 180°.22
Result and Discussion Unit Cell and Space Group Determination. The X-ray fiber diffraction pattern of the clathrate form of
Table 3. Comparison between the Calculated Structure Factors (Fcalc) for the Model of the Clathrate Form of s-PMMS with CS2 of Figure 4 and the Observed Structure Factors (Fobs), Evaluated from the Intensities Observed in the X-ray Fiber Diffraction Pattern of Figure 1a hkl
010 200 210 020 220 400 030 410 230 420 040 240 430 600 620 440 050 450 800 640 111 211 121 311 221 401 321 131 411 231 511 141 521 601 531 621
13.00 8.85 7.14 6.61 5.28
13.10 8.90 7.36 6.55 5.28 4.45 4.37 4.21 3.92 3.68 3.27 3.11 3.07 2.67 2.70 2.64 2.62 2.26 2.23 2.20 6.27 5.35 4.83 4.44 4.37 3.87 3.83 3.73 3.71 3.50 3.14 2.98 2.90 2.77 2.60 2.55
101 29 74 91 49 115 56 54 87 34 56 9 67 25 95 5 82 36 1 43 77 30 84 161 53 99 23 117 71 21 41 48 28 25 43 41
251 711 541 351 721 821 012 112 202 022 122 312 222 402 322 032 132 412 422 332 512 042 522 432 242 532 622 442 052 152 252 712 632 542 352
4.40 3.92 3.30 3.10 2.91 2.65 2.22 6.24 4.87 4.40 3.77
} } }
136 97 50
52 75 108
3.60 3.38 3.15 2.91
2.39 2.37 2.30 2.29 2.27 2.03 3.74 3.66 3.57 3.35 3.29 3.16 3.14 2.93 2.92 2.91 2.87 2.86 2.68 2.61 2.58 2.51 2.44 2.43 2.41 2.25 2.22 2.18 2.17 2.16 2.11 2.10 2.08 2.05 2.04
27 33 55 8 53 25 34 6 53 71 33 121 50 102 37 37 7 43 75 25 31 28 34 26 33 38 80 31 52 19 10 35 22 49 25
} } }
a The Bragg distances, observed in the X-ray fiber diffraction pattern and calculated for the proposed orthorhombic unit cell with axes a ) 17.8 Å, b ) 13.1 Å, and c ) 7.8 Å, are also shown. An occupancy factor of 0.7 has been considered. Reflections not observed with Fcalc less than 20 have not been reported.
Macromolecules, Vol. 36, No. 3, 2003
Figure 6. Projections along c and a axes of the packing models proposed for the s-PS clathrate form containing I2 (a, d),5 the s-PPMS clathrate containing THF (b, e),14 and of the clathrate of s-PMMS containing CS2 (c, f). The approximated z/c fractional coordinates of the barycenters of the phenyl rings are shown. R ) right-handed, L ) left-handed helices. In (d, e, f) only a couple of polymer chains along the b axis are reported.
s-PMMS containing CS2 is reported in Figure 1 while the list of the observed reflections for the same sample is reported in Table 1. The data in Table 1 can be well indexed in terms of an orthorhombic unit cell with cell constants a ) 17.8 Å, b ) 13.1 Å, and c ) 7.8 Å. Assuming two s(2/1)2 polymer chains (eight monomer units) and four CS2 molecules per unit cell, the calculated density is 1.14 g/cm3. This value has to be compared with the experimental densities, measured by flotation, on freshly prepared unoriented clathrate samples presenting a diffraction pattern coherent with the fiber diffraction patter shown in Figure 1 and on amorphous samples, which give both a mean value of 1.02 g/cm3. The density measurements were done on unoriented clathrate samples because the transformation into form I is much slower that in the case of oriented ones.23 In the hypothesis that all the symmetry elements of the s(2/1)2 chain conformation are maintained in the lattice, we have assumed the space group Pcaa, according to the systematic absence of hk0 and h0l reflections with h ) 2n + 1 observed in the X-ray diffraction pattern. Chain Conformation and Packing Model. At variance with the clathrate forms of s-PS and s-PPMS, for which only one s(2/1)2 conformation is possible for the chains (right- and left-handed), the presence of the methyl group on the benzene ring in the meta position leads to the two different conformations with this
symmetry sketched in Figure 2a,b. In addition to these, we have also considered a third (statistical) conformer with symmetry s(2/1)/2 obtained by a combination of the two different conformers previously described, in which two methyl groups, having each an occupancy factor equal to 0.5, are positioned in the meta position of every phenyl group. In the space group Pcaa there are, for each of these conformations, only two different ways of packing the chains in the unit cell, which differ from each other for a rotation by 90° of the chains around their axes and a translation along z of 1/4c. For only one of the six obtainable models a good packing of the chains is achieved, and there is the required space along the b axis for the inclusion of two molecules of CS2. The ab projection of this model is reported in Figure 3. Subsequently, we have positioned the CS2 molecule 3.6 Å far from the chain axis with its molecular axis parallel to the a axis of the cell and with its 2-fold symmetry axis, perpendicular to the S-S direction, coincident with the crystallographic 2-fold axis at z ) 0. The packing has been then refined using Cerius2 minimization procedures in which both packing and chain conformation have been varied at the same time. After minimization, the chain conformation remained substantially unchanged, while the guest molecule was rotated a few degrees around its 2-fold axis of and its center of gravity was translated at 3.76 Å from the chain axis. The model of packing corresponding to the mini-
Petraccone et al.
Macromolecules, Vol. 36, No. 3, 2003
mum of energy is reported in Figure 4a,b. In the resulting model all the contact distances between nonbonded atoms are greater than 4 Å with the exceptions indicated in Figure 4, all relative to interactions between the guest molecule and chains. Considering only s-PMMS adjacent chains, the smallest distances are 4.11 Å along a and 4.25 Å along b. For this model the discrepancy factor R was about 23%. To improve the agreement, we have considered two possibilities. At first, we have varied the position and orientation of the guest molecules and also considered the possibility of a small positional disorder for them. These attempts did not improve in a significant way the agreement, but only introduced worse distances between nonbonded atoms. In a second time, we considered the possibility of the presence of some vacancies in the cavities by introducing a degree of occupancy for the CS2 molecules as already done in the case of the s-PS clathrate containing I2.5 The discrepancy factor R vs the degree of occupancy shows a minimum for an occupancy factor ≈70% of the guest molecules, as apparent from Figure 5. For this occupancy factor the calculated density is equal to 1.06 g/cm3. This result partially justifies the large difference between the observed and calculated densities discussed in ref 23. The fractional coordinates of an asymmetric unit of the model proposed are listed in Table 2. Table 3 compares the calculated and the observed structure factors; the final discrepancy factor R is 16%.
o-DCB, give rise to R class clathrates, while smaller molecules, such as THF, give rise to β class clathrates.18 It is evident from Figure 6 that the clathrate form of s-PMMS presented in this work is characterized by cavities hosting the guest molecules typical of the β class. As far as the packing of the helices along the a axis is concerned, the chains are packed in such a way to realize a close packing similar to that found along the a axis of the clathrate forms4-6 and of the δ form8 of s-PS (cf. Figure 6a,c), in which the distances between chains vary from 8.5 to 8.8 Å, similar to that found for our case that is 8.9 Å. On this basis the presence of the methyl groups in the meta position seems to be not critical as far as the approach of the chains along the a axis is concerned. Finally, it is worth noting that molecules having similar shape and symmetry, as I2 and CS2, which nest in the single s(2/1)2 helical chain in an analogous way (cf. Figure 6d,f), give rise to two clathrates of different class, R for s-PS and β for s-PMMS, respectively. To explain this different behavior, molecular mechanics calculations are in progress.
References and Notes
In the present paper, the clathrate crystalline form of syndiotactic poly(m-methylstyrene) containing CS2 has been obtained and its crystalline structure has been determined. The structure is characterized by polymer chains in s(2/1)2 helical conformation and CS2 molecules packed in an orthorhombic unit cell with axes a ) 17.8 Å, b ) 13.1 Å, and c ) 7.8 Å, according to the space group Pcaa. The calculated crystalline density is 1.14 g/cm3 for two polymer chains and four carbon disulfide units per cell. In Figure 6 the crystalline structures of the s-PS clathrate containing I25 (Figure 6a,d), the clathrate form of s-PPMS containing THF14 (Figure 6b,e), and the clathrate form of s-PMMS containing CS2 (Figure 6c,f) are compared. The structure of the clathrate represented in Figure 6a,b can be considered as representative, as far as the packing of the chains is concerned, of all known clathrate structures of s-PS4-6 and of the δ form8 of this polymer. In this case, the cavities in which the guest molecules are hosted are located around a crystallographic inversion center and are formed by enanthiomorphous chains, belonging to different close packed layers stacked along the b axis of the cell. Clathrates showing this kind of cavity have been indicated as R class clathrates.18 The clathrate form of s-PPMS containing THF (Figure 6b,e), instead, is representative of a second type of clathrate, shown for the first time for this polymer, and classified as β class clathrates, in which the cavities are formed by four benzene rings of one polymer chain and two benzene rings of the adjacent isomorphous chain. For this polymer also R class clathrates have been described, similar to those formed by s-PS, and has been clearly pointed out that the choice of the class for s-PPMS depends strictly on the steric hindrance of the guest molecules. In particular, large molecules, such as
(1) (a) Ishihara, N.; Seimiya, T.; Kuramoto, M.; Uoi, M. Macromolecules 1986, 19, 2464. (b) Zambelli, A.; Longo, P.; Pellecchia, C.; Grassi, A. Macromolecules 1987, 20, 2035. (2) (a) Ishihara, N.; Kuramoto, M.; Uoi, M. Macromolecules 1988, 21, 3356. (b) Resconi, L.; Albizzati, E.; Giannini, U.; Giunchi, G.; Mazzocchi, R. Italian Patent Application 22827 A, 1986. (c) Grassi, A.; Longo, P.; Proto, A.; Zambelli, A. Macromolecules 1989, 22, 104. (d) Pellecchia, C.; Longo, P.; Grassi, A.; Ammendola, P.; Zambelli, A. Makromol. Chem., Rapid Commun. 1987, 8, 277. (3) (a) Immirzi, A.; de Candia, F.; Ianelli, P.; Zambelli, A.; Vittoria, V. Makromol. Chem., Rapid Commun. 1988, 9, 761. (b) Vittoria, V.; de Candia, F.; Iannelli, P.; Immirzi, A. Makromol. Chem., Rapid Commun. 1988, 9, 765. (c) Guerra, G.; Vitagliano, M. V.; De Rosa, C.; Petraccone, V.; Corradini, P. Macromolecules 1990, 23, 1539. (d) Chatani, Y.; Shimane, Y.; Inoue, Y.; Inagaki, T.; Ishioka, T.; Ijitsu, T.; Yukinari, T. Polymer 1992, 33, 488. (4) Chatani, Y.; Inagaki, T.; Shimane, Y.; Iijtsu, T.; Yukimori, T.; Shikuma, H. Polymer 1993, 34, 1620. (5) Chatani, Y.; Shimane, Y.; Inagaki, T.; Shikuma, H. Polymer 1993, 34, 4841. (6) De Rosa, C.; Rizzo, P.; Ruiz de Ballesteros, O.; Guerra, G.; Petraccone, V. Polymer 1999, 40, 2103. (7) Guerra, G.; Milano, G.; Venditto, V.; Musto, P.; De Rosa, C.; Cavallo, L. Chem. Mater. 2000, 12, 363. (8) De Rosa, C.; Guerra, G.; Petraccone, V.; Pirozzi, P. Macromolecules 1997, 30, 4147. (9) Guerra, G.; Manfredi, C.; Rapacciuolo, M.; Corradini, P.; Mensitieri, G.; Del Nobile, M. A. Ital. Pat. 1992 (C.N.R.). (10) Iuliano, M.; Guerra, G.; Petraccone, V.; Corradini, P.; Pellecchia, C. New Polym. Mater. 1992, 3, 133. (11) De Rosa, C.; Petraccone, V.; Guerra, G.; Manfredi, C. Polymer 1996, 37, 5247. (12) Dell’Isola, A.; Floridi, G.; Rizzo, P.; Ruiz de Ballesteros, O.; Petraccone, V. Macromol. Symp. 1997, 114, 243. (13) De Rosa, C.; Buono, A.; Caporaso, L.; Petraccone, V. Macromolecules 2001, 34, 7349. (14) Petraccone, V.; La Camera, D.; Pirozzi, B.; Rizzo, P.; De Rosa, C. Macromolecules 1998, 31, 5830. (15) Petraccone, V.; La Camera, D.; Caporaso, L.; De Rosa, C. Macromolecules 2000, 33, 2610. (16) La Camera, D.; Petraccone, V.; Artimagnella, S.; Ruiz de Ballesteros, O. Macromolecules 2001, 34, 7762.
Acknowledgment. This work was supported by the Ministero dell’Universita` e della Ricerca Scientifica e Tecnologica (PRIN 2000 titled “Selective polymerization: coordination catalysts and control of physical properties of the resulting polymers”).
Macromolecules, Vol. 36, No. 3, 2003 (17) Loffredo, F.; Pranzo, A.; Guerra, G.; Venditto, V.; Longo, P. Macromol. Symp. 2001, 166, 165. (18) La Camera, D.; Petraccone, V.; Artimagnella, S.; Ruiz de Ballesteros, O. Macromol. Symp. 2001, 166, 157. (19) Cromer, D. T.; Mann, J. B. Acta Crystallogr. 1968, A24, 321. (20) Sun, H. J. Phys. Chem. B 1998, 102, 7338. (21) De Rosa, C.; Auriemma, F.; Esposito, S.; Buono, A. Polymer, in press (personal communication). (22) Interatomic Distances Supplement. Special Publication No. 18 Supplement 1956-1959; The Chemical Society: London, 1965. (23) We are aware of the substantial difference between calculated and experimental densities. Nevertheless, we believe that this discrepancy is not detrimental for the structural investigation. In fact, some of us have already found, in the case of the clathrate form of s-PPMS containing THF, similar differences between the calculated density for the crystalline
structure (1.13 g/cm3) and the experimental density of the semicrystalline sample (1.02 g/cm3).14 In that paper were also presented experimental evidence explaining, at least in part, this difference. As a matter of fact, we have frequently observed that clathrate semicrystalline samples may have densities equal to completely amorphous samples, or even lower. This fact may be attributed to a microporous nature of the amorphous regions of the clathrate specimens that, left in open air, show the tendency to lose guest molecules from the amorphous regions more rapidly than from the crystalline regions. It is worth noting that TGA measurements on our unoriented semicrystalline samples show a CS2 content not higher than 14%, indicating, on the basis of the proposed structural model, that the amorphous regions of the specimens contain less solvent of the crystalline regions.